Large Piezoelectric Response in Hybrid Rare-Earth Double Perovskite Relaxor Ferroelectrics.
Shi, Chao; Ma, Jia-Jun; Jiang, Jia-Ying; Hua, Miao-Miao; Xu, Qi; Yu, Hui; Zhang, Yi; Ye, Heng-Yun; Journal of the American Chemical Society 142 (2020) 9634–9641; doi:10.1021/jacs.0c00480

data_4134869
_publ_section_title
;
 Large Piezoelectric Response in Hybrid Rare-Earth Double Perovskite
 Relaxor Ferroelectrics.
;
_journal_issue                   21
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9634
_journal_page_last               9641
_journal_paper_doi               10.1021/jacs.0c00480
_journal_volume                  142
_journal_year                    2020
_chemical_absolute_configuration syn
_chemical_formula_sum            'C16 H34 La N8 O20 Rb'
_chemical_formula_weight         882.89
_space_group_crystal_system      cubic
_space_group_IT_number           198
_space_group_name_Hall           'P 2ac 2ab 3'
_space_group_name_H-M_alt        'P 21 3'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2017/1
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.502
_cell_length_b                   14.502
_cell_length_c                   14.502
_cell_measurement_reflns_used    45516
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.0520
_cell_measurement_theta_min      1.9710
_cell_volume                     3049.887
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.968
_diffrn_measurement_device_type  'rigaku saturn 724'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0664
_diffrn_reflns_av_unetI/netI     0.0196
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.968
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            101302
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.949
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         32.012
_diffrn_reflns_theta_min         1.986
_exptl_absorpt_coefficient_mu    3.083
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.61852
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.923
_exptl_crystal_description       block
_exptl_crystal_F_000             1760
_exptl_crystal_size_max          0.17
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.853
_refine_diff_density_min         -1.284
_refine_diff_density_rms         0.180
_refine_ls_abs_structure_details
;
 Flack x determined using 1187 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.005(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.231
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         3376
_refine_ls_number_restraints     19
_refine_ls_restrained_S_all      1.228
_refine_ls_R_factor_all          0.0604
_refine_ls_R_factor_gt           0.0537
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0713P)^2^+2.3638P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1398
_refine_ls_wR_factor_ref         0.1426
_reflns_Friedel_coverage         0.781
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.926
_reflns_number_gt                3055
_reflns_number_total             3376
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja0c00480_si_002.cif
_cod_data_source_block           (RM3HQ)2RbLa(NO3)6-T293K
_cod_depositor_comments
'Adding full bibliography for 4134868--4134872.cif.'
_cod_original_cell_volume        3050.2
_cod_database_code               4134869
_shelx_shelxl_version_number     2017/1
_shelx_res_checksum              65737
_shelx_hkl_checksum              96038